International Journal of Material Science

IJMSCI

Modeling of Radar Absorbing Materials Using Winning Particle Optimization Applied on Electrically Conductive Nanostructured Composite Material Davide Micheli, Roberto Pastore, Mario Marchetti Depart ment of Astronautic, Electric and Energy, Sapienza Un iversity of Ro me Ro ma, Italy davide.micheli@uniro ma1.it; roberto.past@gmail.co m; mario.marchetti@uniro ma1.it Abstract- Modelling and manufacturing of radar absorbing material are proposed using multilayer composite nanostructured materials and the recently introduced winning particle optimization algorithm. The study concerns tile of materials with dimensions of 0.3m×0.3m made of nanostructured composite materials, which consist on epoxy-resin and industrial grade carbon nanotube (CNTs) fillers. The industrial grade CNTs were appositely chosen for their low costs, in order to be applied in great amount to build large tile of composite materials. Here modelling takes into account for an extended frequency band (5 to 18 GHz), for several incidence angles of the electromagnetic field (0 to 80°), and for the minimization of the electromagnetic reflection coefficient. At last simulations are compared with measurements of reflection coefficient. Despite some errors mostly due to the manufacturing process, simulations are in good agreement with measurements, showing an interesting approach to design multilayer radar absorbing materials. KeywordsRadar Absorbing Materials; Evolutionary Computation; Winning Particle Optimization; Modeling; Carbon Nanotubes; Composite Nanostrucutred Materials; Layered Structures; Non-Destructive Testing; NRL-Arch; Stealth

I. INT RODUCTION Radar absorbing materials (RAM) acquired importance since their first applications in military field [1-6]. Germany pioneered the first aircraft to use RAM during World War II, in the form of the “Horten Ho 229”, in order to reduce the radar signature, and concerned with radar camouflage for submarines, developed “Wesch” material, a carbonyl iron powder loaded rubber sheet about 0.3 inches thick and a resonant frequency at 3 GHz. Co mposite materials considered in this work are based on epoxy matrix reinforced with carbon nanomaterials. These latter were chosen taking into account their good microwave absorption behaviour [7] and the low market p rices. In fact, the economic aspects, normally neglected in small laboratory applications, are important in real applicat ions where the amount of carbon nanopowders fillers could be relatively high. In such scenario, a good compro mise in terms of cost/performances was obtained using industrial grade mu ltiwall carbon nanotubes (MWCNTs) with a cost of about 300 $/ kg. MW CNTs with co mmercial name o f NANOCYLTM NC7000 (diameter around 9.5 n m, length 1.5 µm, purity 90%) were bought at NANOCYL. Bi-co mponent Epo xy-resin PrimeTM 20LV (density 1.123 g/cm3 ) with Hardner (density 0.936 g/cm3 ) was used as matrix. RAM is based on layered materials where each layer is made of carbon nanostructured composites materials in d ifferent weight percentages. The recent developed winning particle optimization search

algorith m (WPO) was applied in order to design and optimize mu ltilayer materials able to effectively absorb microwaves in the range 5 GHz to 18 GHz. The paper is organized in 5 distinct sections. In Section II, mathematical model of absorber is shown; in Section III, WPO is described; in Section IV, numerical design of RAM is d iscussed and in Section V, RAM manufacturing and electro magnetic performance co mparisons between simulation and manufactured RAM are shown. In this section the adopted experimental setup is accurately described showing the NRL-arch test fixture. It is crucial to highlight the interdisciplinary research activity through nanomaterials, electro magnetic wave propagation theory, composite materials manufacturing techniques and search computation algorithms. All of them are required to design the “quasi perfect absorber”. II. RAM MATHEMATICAL MODEL WPO algorith m [8-9], has been applied to solve a quite complex p roblem consisting in the design and optimization of micro wave absorbing mult ilayer materials. Optimized RAM is based on nanomaterials in particu lar carbon nanostructured composites materials. Conductive fillers have been uniformly dispersed in an epo xy resin at d ifferent weight percentages (0.5, 1, 2, 2.5, 3 wt %). In Table I, six different composite materials and the index code adopted by WPO to identify each material are shown. TABLE I CODING OF MATERIALS IN THE DATA BASE

Materials Epoxy- Resin

Materials Code 1

MWCNT , 0.5 wt%

2

MWCNT , 1.0 wt%

3

MWCNT , 2.0 wt%

4

MWCNT , 2.5 wt%

5

MWCNT , 3.0 wt%

6

The resulting composites samples have been dielectrically characterized in a previous work [10-11] by waveguide measurements to recover the dielectric p roperties of the composite materials in the data base (DB). In this paper the DB of these dielectric parameters as function of frequency is used to supply the WPO modeling algorith m. In Tab le II, a brief summary of the dielectric permittiv ity of composite materials at 6GHz, 12 GHz, 18 GHz, is shown. After that, numerical simu lations of RAM have been carried out. In particular, electro magnetic analysis has been performed integrating the

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 31 ~

International Journal of Material Science

IJMSCI

forward/backward propagation formalism to the in-house built WPO, thus able to carry out optimization upon oblique incidence angles over a fin ite angular range. TABLE II DIELECTRIC P ERMITTIVITY OF COMP OSITE NANOSTRUCTURED MATERIALS

Materials Re al Part and Imaginary Part F1= 6 Ghz

F2= 12 Ghz

F3=18 Ghz

In RAM applications, RC at the air-absorber interface can be evaluated by the follo wing equation relating the free space impedance to the input impedance seen at the air-mult ilayer structure interface

Epoxy- Resin

3.11

0.10

3.07

0.08

3.07

0.08

MWCNT , 0.5 Wt%

5.52;

0.90

5.33

1.81

5.21

2.83

MWCNT , 1.0 Wt% MWCNT , 2.0 Wt%

9.52 11.42

5.27 6.89

6.75 8.82

2.88 4.48

5.39 7.45

1.95 3.38

MWCNT , 2.5 Wt%

12.90

11.28

10.86

10.35

9.71

9.79

MWCNT , 3.0 Wt%

18.21

14.50

17.29

13.65

16.72

13.31

RC TM / TE =

The developed code min imizes reflection and transmission coefficients under the thickness min imization constraint. Finally, broadband quasi-perfect absorbers in the band 5-18 GHz are achieved combin ing the filler families, i.e., exhib iting a loss factor (LF%) greater than 90% in most of the band, for thicknesses ranging between 5 and 12 mm. Main goal of design and optimization work was to achieve values (< -10 d B) of reflection coefficients (RC), for angular apertures within 40° in the most part of the frequency band. The design/optimizat ion is basically a minimization procedure which seeks the best tradeoff between structure thickness (to be minimized) and absorbed EM power (to be maximized). The absorbing power has been quantified through the so-called “loss factor” LF%, defined as follows [10-11].

(

2

LF % = 1 − RC − TC

2

)⋅100.

As far as geometric properties of multilayer structures are concerned, thickness of each layer can range fro m 0 to 10 mm, while the number of layers is upper-bounded to maximum 10 layers. The effective nu mber of layers is established by the WPO optimizat ion procedure which is able to remove one or more useless layers from the mult ilayer structure. The order of layer materials is not a priori fixed; instead WPO algorithm decides which material need to be used for each layer.

Z iTM / TE − Z 0TM / TE Z iTM / TE + Z 0TM / TE

TM / TE RC dB = 20 Log 10

,

(3)

Z iTM / TE − Z 0TM / TE Z iTM / TE + Z 0TM / TE

where Z0 ≅ 377 Ω is the free space impedance and Zi is the input impedance at the first air-absorber interface. The input wave impedance of the mult ilayer, backed by PEC, can be expressed iterating the following equation for x-th-layer [1113].

Z ixTM / TE = η xTM / TE

Z ixTM−1 / TE cos(k x t x ) + jη xTM / TE sin (k x t x ) (4) η xTM / TE cos(k x t x ) + jZ ixTM−1/ TE sin (k x t x )

In (4), tx = y x-1 -y x is the x-th layer thickness expressed in m, whereas the wave number kx of each layer along y axes is k x2 = (2π f ) µ 0 ε 0 µ rx ε rx cos 2 ϑ x = 2

(1)

(

= (2π f ) µ 0 ε 0 µ rx ε − jε 2

' rx

'' rx

)cos

(5) 2

ϑx

In RAM systems the transmission coefficient TC=0 (because of the perfect electric conductor (PEC) layer at the end of the mult ilayer), and the RC is the WPO-optimized reflection coefficient.

where f is frequency of the incident electro magnetic wave in Hz,ε’ is the real part o f x-th-layer permittivity and ε” is the imaginary part o f layer permittiv ity.

Both are expressed in the linear form. LF% physical mean ing is related to the fraction of the incident power vanishing inside the materials because of localizat ion and dissipation phenomena. Since the calculation of RC becomes a crucial point for RAM optimizat ion goal, a rigorous approach for co mputing reflected waves at each layer has been adopted [11-13].

Co mplex waves appear in oblique incidence and lossy dielectrics problems [13]. Because of the wave number become complex-valued, e.g., k= β − jα , the angle of refraction and possibly the angle of incidence may become co mp lex-valued too. In calculat ing k x by taking square root of (5), it is required, in co mplex-wave problems, to get the correct signs of their imaginary parts, such that evanescent waves are described correctly. This leads to define an "evanescent" square root as

Both normal and oblique incidences have been evaluated during the automatic optimizat ion. In Fig. 1, a general scheme of the electro magnetic absorbing mult ilayer structure is presented. Each layer is generally denoted by index x.

E x++1

εx+1 µ x+1 Air

E x−+1

θx yx θ x+1

Incident EM Field

x+1

εx µx

ηx

Tx

εx-1 µ x-1 θ x-1

follows. Let = ε rx

' rx

− jε rx ''

) with

'' ε rx > 0 for an absorbing

med iu m, then

(

) ( )

(2π f )2 µ ε µ ε ' − jε '' cos 2 ϑ , if ε '' > 0 0 0 rx rx rx x rx (6) k x2 = 2 ' 2 '' − j − (2π f ) µ 0 ε 0 µ rx ε rx cos ϑ x , if ε rx = 0

PEC

Since all nanostructured composite materials availab le in

y

y x-1

(ε

the DB are with ε rx'' > 0 then kx is as usually computed.

ηx-1 T x-1

III. WINNING PART ICLE OPTIMIZATION Zix

Zix-1

x

x-1

1

0

Fig. 1 General Multilayer scheme of electromagnetic absorbing structure; in RAM systems the back layer is a perfect electric conductor (PEC).

WPO is a simp le algorith m where at each t ime epoch of evolution, the particle, which best fit the objective function, is deputed to pilot the trajectory of the remaining particles within the multid imensional space of solutions, i.e., variables to be optimized. In Fig. 2, WPO flow chart is shown. At the

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 32 ~

International Journal of Material Science

IJMSCI

beginning of the iterations, particles are rando mly d istributed within the n-d imensional search space. Start WPO Algorithm Initial random particles generation

between the current particle mth-coordinates and the best particle mth-coordinates. Here, q is the index of the best particle found in each iteration and the condition wh ich needs to be grant is q≠k, i.e., all kth particles can be displaced except the best qth particle. Equation (7) describes the mentioned approach. Particle position at the (i+1)th iteration as a function of particle position in the previous ith iteration is .

Pmk (i + 1) = δ Rm Pmk (i ) + g PBmq (i )

Particles Pi fitness evaluation

where g = +1 if Pmk (i ) < PBmq (i )

M ark the best particle (BPq) with q-index ranging from 1 to max particles number

g = −1 if Pmk (i ) > PBmq (i ) k = Particle index in the range [1 , Particle Number] q = Best Particle index in the range [1 , Particle Number] and k ≠ q m = ranges in [1 , n] n = Space Dimensions Rm = random number in the interval [0 , 1] δ = Convergence Parameter i = current iteration in the range [1, N] N = Number of iteration Rm is used to randomly define the amount of displacement of each single coordinate. Such randomization develops the searching ability by conferring some causality to the amplitude of ju mps. Convergence parameter δ helps the final convergence of the WPO algorith m as follows. At the beginning of the iterations, the WPO must be capable to exp lore the largest space of solutions as possible. On the other hand, close to the end of the iterations, high amp litude of ju mps could represent a drawback since a position representing the optimal solution could forbid. In order to imp rove the WPO convergence, a mechanis m provid ing a progressive reduction of “maximu m ju mps amp litude” has been introduced and it is identified by the δ parameter. Calling N the total number of iterations and supposing ith the current iteration, then the value of δ is given by

Extraction of all m-coordinates of each particles in the n-dimensional space

no

Pmk < PBmq k ≠ q, m=1:n

Pmk = δ Rm Pmk − PBmq

yes

Pmk = δ Rm Pmk + PBmq

M utation operation for some randomly position coordinates m of the particles P k ≠ PB q m

m

Check of boundary conditions for each single m-coordinate

no

(7)

δ = σ 1 −

yes Iteration end ?

i N + 1

S

σ = J (Rm − 0.5)

End WPO Algorithm Fig. 2 WPO flow chart

At each iteration time, the objective function of each particle is computed. Then, particles are compared to each other using value of their objective function and the best fitting particle is marked with its proper index. Each part icle position is comp letely defined by its coordinates and their number represents the dimension of the space where all part icles ju mp searching for the optimal solution. Trajectory of each particle, except that of the best fitting particle, is defined in the following way: if mth-coordinate of a certain part icle Pk is lesser then the corresponding mth-coordinate of the current best particle PBq , then the new mth-coordinate will result fro m the sum of current part icle and best particle mth-coordinates; while if mth-coordinate of a certain particle Pk is greater than the corresponding mth-coordinate of the current best particle PBq , then the new mth-coordinate will result fro m the difference

(8) (9)

where J is the “ju mp amplitude” defined by the user as a numerical parameter in the main program of WPO, in this scenario it has been valued to 3 after several t rials to assure a good performance in do main solution explorat ion. In (8), the meaning of σ and S parameters is in fast or slow convergence of the WPO algorith m. In part icular, the h igher the σ, the greater the init ial ju mps amp litude and the greater the distances where particles will start to explore the search space. As far as S is concerned the higher its value, the faster the convergence to a suboptimal solution. The parameter σ is made using J and Rm such that (Rm - 0.5) is a random number between [−1/ 2, +1/2]. The random part o f σ develops the search capability of the algorithm. Even though mutation operation has not been applied on the subsequent reported optimizations (mutation=0%), it has to be noticed that mutation can be included in WPO algorithm to further increase the random search capability. At the end of each WPO iteration, checking of boundary conditions for the new set of particles coordinates

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 33 ~

International Journal of Material Science

IJMSCI

is computed in order to avoid overcoming the constraints. The entire loop cycle can be iterated several times in order to get the required objective function minimization. IV. RAM DESIGN AND OPTIMIZATION The presented modeling procedure, takes into account for several incidence angles and, the design/optimization procedure can be forced to run for a one particular incidence angle or for a range of angular incidences where the global objective function has to be optimized. In particular the incidence angles here range between 0° and 80° with step 10°. As far as layer materials are concerned each one can be chosen among all of different manufactured composite materials. In Table I, all the composite materials available in the DB are reported and each composite material has been coded using an integer number. WPO can access to DB in order to allocate the most appropriate materials for each layer of the mult ilayer RAM. In WPO procedures the modeling functions are called by the main program to co mpute: materials intrinsic impedances, inoutgoing refraction angle, TE/TM layer wave impedance, reflection coefficient (RC), and the loss factor (LF). The mu ltilayer absorbing structures considered in the design procedure can have up to 10 layers so dimensionality of layer space is 10 i.e., m = 10, 9. . . 1. Since the optimization are for both: layer thickness and layer material type then WPO algorith ms need to be structured in order to take into account for both quantities.

[

]

k In WPO algorith m we have: T k (i ) = t10 (i ), t9k (i ),......., t1k (i ) , as array of thicknesses, where Tmk (i ) is the thickness of m-th

[

]

k layer, and P k (i ) = p10 (i ), p9k (i ),......., p1k (i ) , as array of material k type, where Pm (i ) is the type of material associated to the mth layer.

implementation, the value of convergence parameter S is set to 1. WPO try to minimize a global objective function (GOF) which in turn is built using elementary objective functions (EOF). The EOF for TM and TE modes are named as CostRCTM , CostRCTE , for reflection coefficient. The formal definit ion of the EOF for TM and TE modes are shown in (12),(13),(14). We can observe that for each part icle (Pa), the corresponding EOF is evaluated over the entire frequency band and over the entire incidence angular range, adopting frequency and angular steps chosen by the user before starting the WPO, freq = f max ϑ =ϑ max CostRCTM (Pa ) = ∑ ∑ RCTM (Pa, freq, ϑ ) (12) freq = f min ϑ =ϑ min

freq = f max ϑ =ϑ max CostRCTE (Pa ) = ∑ ∑ RCTE (Pa, freq, ϑ ) freq = f min ϑ =ϑ min where Pa is the current particle, freq is the frequency step, fmin and fmax is the frequency band start and stop, θ is the current angular step, θmin and θmax represent the angular range bounds. The definit ion of the EOF for thickness is

CostT (Pa ) = [t10 ( Pa ) + t9 ( Pa ) + .... + t1 ( Pa )] (13) where tm is the thickness of the m-th layer. A weighting factor called α ranging in (0<α<1), weight CostT w.r.t. CostRC. Such weighting factor is chosen by the user and its meaning have to be intended as the capability of the tool to design the multilayer structure making privilege to the electro magnetic perfo rmances w.r.t. the thickness when αis close to 1. Final GOF is a linear co mbination of the described EOFs, (14) GOF (Pa ) = α OF1(Pa ) + (1 − α ) OF 2(Pa ) where CostRCTM (Pa ) CostRCTE (Pa ) + OF 1(Pa ) = A A CostT (Pa ) OF 2(Pa ) = B

The equations related to layer thicknesses and layer material for each single part icle are simp ly updated according to,

Tmk (i + 1) = δ Rm1 Tmk (i ) + g Thickness TBmq (i ) Pmk

(i + 1) = round (δ

Rm 2 Pmk

(i ) +

g Material PBmq

(i ))

(10)

Where, Rm1 and Rm2 are random numbers in the closed range 0-1, Tmk (i ) is the current kth-particle, mth-layer-

thickness at the ith-iteration, wh ile Pmk (i ) is the current kthparticle, mth-layer-material at the ith-iteration. Rounded values in material equation are required since the index of material of each layer must be an integer number ranging fro m 1 to the number of materials availab le in the DB of materials. q gThickness = +1 if T k (i ) < TB (i ) m m (11) q gThickness = −1 if T k (i ) > TB (i ) m m q k g Material = +1 if P (i ) < PB (i ) m m q g Material = −1 if P k (i ) > PB (i ) m m

where q is the index of best particles TB and PB; k is the index of particles with k ≠ q; n is the dimension number; m is the current dimension ranging between [1,n]. In the presented

A and B are normalization factors: A is the product between the frequency step number and the angle step number, whereas B is the product between the maximu m layer number and the maximu m layer thickness. In the follo wing subsection two RAM models are shown. A. RAM First Simulation In the first RAM simulat ion a weighting factor α=0.9 returned the scheme of layered material shown in Fig. 3. The electro magnetic wave imp inges upon the first layer made of epo xy-resin. Incidence and reflection angle is called θ 0 , ranging fro m 0° to 80°. Total thickness of mu ltilayer RAM is 11.77 mm and the final nu mber of layers is 4. Tile is composed on the top by the lowest lossy material (epo xy-resin) as the first layer up to the h ighest lossy material in the DB (MWCNTs 3 wt%) as third layer backed by PEC. This structure can be viewed as a graded lossy system in the first three layers and a resonant structure in the fourth layer, where the chosen materials are not the highest lossy materials (MWCNTs 0.5% wt). In particu lar graded lossy systems are composed by a quasi-wave impedance matched material where the first interface between free space and epoxy-resin is the best coupling material ab le to assure the lowest reflection

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 34 ~

International Journal of Material Science

IJMSCI

coefficient at the first air-absorber interface. MWCNTs 1wt% and MWCNTs 3wt% instead have lower characteristic wave impedances and greater losses with respect to epoxy-resin and as a consequence they are placed in sequence in the layers order. Incidence Wave

Reflected Wave

θ°

Infinite length = 3.05 mm

Infinite length

= 2.39 mm Resin-epoxy

= 4.81 mm

MWCNTs 1wt%

= 1.02 mm

MWCNTs 3wt% MWCNTs 0.5wt% Perfect Electric Conductor ∼11.77 mm

Fig. 3 RAM multilayer simulated: Resin-epoxy, MWCNTs 1wt%, MWCNT s 3wt%, MWCNT s 0.5 wt%, PEC

In Fig. 4, reflection coefficients TE/TM (dB) are shown. It can be noticed that for normal incidence angles, TE and TM curves coincides whereas around 7, 9, 12, 15 GHz, there are some incidence angles where curves show values of reflection coefficient TM even lower with respect to that at normal incidence. Such angles are denoted as Zenneck angles for lossy materials. theta=0°

-5

100

theta=10°

-10

theta=20°

-15

theta=30°

-20

theta=40°

-25

theta=50°

-30

theta=60°

-35

theta=70°

-40

theta=80°

theta=0° theta=10°

90

theta=20° 80

LossFactor TE %

Module of Reflection Coefficient TM (dB)

0

“impedance matching condition” which in turns is a function of thickness of the absorbing layer. The impedance matching condition takes place when the electro magnetic wave impedance at the first interface between air and RAM is close to that of free space i.e., about 377 Ω. This is why in the simu lation the first layer is logically made of epo xy-resin which possesses the lowest electric permittiv ity and so the higher electro magnetic wave impedance. The electro magnetic wave impedance at the first interface is computed using (4) and depends on dielectric parameter of all materials in the mu ltilayer. The dielectric losses are described by the imag inary part of the permittiv ity (ε") wh ile, thickness of the material is connected to the microwave wavelength within the material. The higher the dielectric losses, the greater are the electro magnetic power dissipation phenomena in the RAM composite material. Unfortunately, usually, the h igher the dielectric permittiv ity, the lower is the electro magnetic wave impedance, wh ich in turn mis match the impedance matching condition with free space [11]. This is why, the RAM is composed of different layers able to progressively match the wave impedance while simultaneously assuring the right dissipation and absorbing behaviour. In Fig. 5, Loss Factor TE/TM is shown. Loss Factor (%) remains above 90% for incidence angles up to 40°. Such values mean that RAM is able to absorb the most part of the electro magnetic field reflecting back only a very little amount of the incoming energy. The extended frequency band 6 to 18 GHz where loss factor is greater than 95%, shows the interesting theoretical performance of this RAM.

theta=30° theta=40°

70

theta=50° 60

theta=60° theta=70°

50 -45 -50

theta=80° 40 6

8

10

12

14

16

18

Frequency (GHz) 30

6

8

-5

theta=10°

-10

theta=20°

-15

theta=30°

-20

theta=40°

-25

theta=50°

-30

theta=60°

-35

theta=70°

-40

theta=80°

10

12

14

16

18

Frequency (GHz)

theta=0°

100

theta=0° theta=10°

90

theta=20° 80

LossFactor TM %

Module of Reflection Coefficient TE (dB)

0

theta=30° theta=40°

70

theta=50° 60

theta=60° theta=70°

50 -45

theta=80° -50

6

8

10

12

14

16

40

18

Frequency (GHz) 30

Fig. 4 RAM Reflection Coefficient (dB) TE and TM

The electro magnetic absorbing capability of a certain material is mainly due to two simultaneous conditions: “dielectric losses” within the composite material and

6

8

10

12

14

16

Frequency (GHz)

Fig. 5 RAM Loss Factor (%) TE and TM

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 35 ~

18

IJMSCI

130

Objective Function minimization

120 110 100 90 80 70 60

0

theta=0°

-5

theta=10° theta=20°

-10

theta=30° -15 theta=40° -20

theta=50°

-25

theta=60° theta=70°

-30 theta=80° -35

6

8

10

12

14

16

18

Frequency (GHz) Module of Reflection Coefficient TM (dB)

In Fig. 6, the asymptotic convergence of WPO evolution is shown. Plot of GOF is shown. The simu lation is made on 800 iterations and 256 searching particles. The time required to complete the computation strongly depends on the amount of particles and iterat ions and by the computer performances in terms of random memory allocation and processing speed. After 600 iterations the behaviour of curve is almost asymptotic showing a probably sufficient convergence of the WPO algorith m in searching the best solution to the RAM design and optimization problem. The computing time also depends on the way in which code is written. Here Matlab has been used. So me procedures were parallelized but others require nested loops of cycle to take into account for particles, frequencies, and incidence angles. These are very time consuming.

Module of Reflection Coefficient TE (dB)

International Journal of Material Science

0

theta=0° theta=10°

-5

theta=20°

-10

theta=30° -15 theta=40° -20

theta=50°

-25

theta=60° theta=70°

-30 theta=80° -35

6

8

10

12

14

16

18

Frequency (GHz) 50 0

100

200

300

400

500

600

700

Fig. 8 RAM Reflection Coefficient (dB) TE and TM

800

Iterations of WPO Algorithm

Fig. 6 WPO evolution and convergence 100

theta=0°

90

LossFactor TE %

B. RAM Second Simulation In the second RAM simulat ion, a lower weighting factor α=0.6 returned the scheme o f layered materials shown in Fig. 7. The mu ltilayer RAM is composed of three different layers, the first one, where the electromagnetic wave arrives, is epoxyresin; the second one is made of MW CNTs at 1wt%, the third layer is made of MWCNTs at 2wt%. The total thickness is about 5.72 mm. In Figs. 8 and 9 the electro magnetic performances of RAM are shown.

theta=10° theta=20°

80

theta=30° 70 theta=40° 60

theta=50°

50

theta=60° theta=70°

40

Incidence Wave

θ°

Reflected Wave

theta=80° 30

6

8

10

12

14

16

18

Frequency (GHz) 100

theta=0°

Infinite length 90

= 0.4132 mm Resin-epoxy

= 2.5176 mm

MWCNTs 1wt% MWCNTs 2wt%

LossFactor TM %

= 2.7958 mm

Infinite length

theta=10° theta=20°

80

theta=30° 70 theta=40° 60

theta=50°

50

theta=60°

Perfect Electric Conductor

theta=70° 40 theta=80°

∼5.72 mm

30

Fig. 7 RAM multilayer simulated: Resin-epoxy MWCNT s 1 wt%, MWCNT s 2wt%, PEC

6

8

10

12

14

16

Frequency (GHz) Fig. 9 RAM Loss Factor % TE and TM

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 36 ~

18

International Journal of Material Science

IJMSCI

The graphs show two peaks of absorption at 0° incidence angle for TE/TM around 7 and 16 GHz. When the incidence angle grows to 50°, 60° and 70° in the TM incidence mode, the first absorption packs shift to 8, 10 and 11 GHz while the second peak disappear.

respect as much as possible the RAM scheme and thickness performed by WPO simulat ion, in the case of Fig. 7. Incidence Wave

Reflected Wave

θ°

Ⅴ. RAM MANUFACTURING AND ELECT ROMAGNETIC

30 cm

PERFORMANCE MEASUREMENT

The second simu lated RAM mu ltilayer scheme has been chosen as the model to try of building a large RAM tile. Each layer was manufactured over the previous using the sample holder as shown in Fig. 10. The manufacturing p rocedure is available in [9]. In Fig. 11, the manufactured RAM tile is shown.

= 3.5 mm

30 cm

= 0.1 mm = 2.5 mm

Resin-epoxy MWCNTs 1wt% MWCNTs 2wt% Perfect Electric Conductor ∼6.1 mm

Fig. 12 RAM multilayer manufactured: Resin-epoxy MWCNTs 1 wt%, MWCNT s 2wt%, PEC

5 Multilayer measurments for normal incidence angle

0

Reflection Coefficient

-5

Fig. 10 Sample holder to build multilayer RAM

-10 -15 TE_0

-20

Multilayer simulation for normal incidence angle

TM_0

-25

TE_90

-30 TM_90

-35

TE_model

-40

TM_model

17.55

16.94

16.33

15.72

15.11

14.51

13.90

13.29

12.68

12.07

11.46

10.86

9.64

10.25

9.03

8.42

7.81

7.21

6.60

5.99

5.38

-45

Frequency (GHz)

Fig. 13 RAM multilayer manufactured: resin-epoxy MWCNT s 1 wt%, MWCNT s 2wt%, PEC

Fig. 11 Final manufactured RAM multilayer tile

The practical realizat ion of the large RAM tile was not easy since the dimensions 30x30 cm required a lot of nanomaterials and the related dispersion process in the epoxy-resin resulted hard. Another very difficult task was to respect the thickness of each layer because the manually ho memade deposition of each layer above the other one caused errors in the value of thickness and in the homogeneity of layers along the surface. The great manufacturing problems rose with the layer made of MWCNTs at 2wt%. In fact, such composite doesn’t remain enough viscous so tile manufacturing process is quite difficult, especially for respect thickness constraints. At the end, the final manufactured mult ilayer RAM is lightly different with respect to the initial simu lation reported in Fig. 7. In Fig. 12 the manufactured RAM mu ltilayer tile scheme is shown. The total thickness of tile is about 6.1 mm. The simu lation of such new tile is shown in Fig. 13. Observing the simu lation it can be highlighted that even small variations of thickness layers are able to affect the reflection coefficient lowering the absorption properties of RAM. This is why it is very important to try to

To evaluate the electromagnetic reflectivity, a NRL arch measurement (bistatic reflect ion method), has been used [14]. In this configuration, t wo antennas are placed for transmitting and receiving signals respectively and the microwave reflectivity at different incident angles can be measured. Using this configuration, the reflection properties of materials, can be measured for different incident angles. It should be noted that in bistatic reflection measurements, the reflection is dependent on the polarization of the incident wave. Incident waves with parallel and perpendicular polarizat ion usually result in different reflect ion coefficients. Besides, special calibration is needed for free-space bistatic reflection measurements [14]. In Fig. 14 bistatic measurement system and the tile in co mposite material is shown. Bistatic measurement system is here based on Agilent software 8571E (material measurement), and Agilent PNA-L vector network analyser. Antenna used are SATIMO Dual Ridge Ho rn SH2000 covering the frequency range 2 – 32 GHz. After the calibration of the NRL bistatic system, the reference in reflection coefficient has been taken adopting only metal p late i.e., without RAM tile. After that measurement of a known sample consisting in ECCOSORB AN73 absorber [7], has been performed in order to be aware about errors in the NRL measurement setup. Confidence of measurements was within 2 d B of interval with respect to reflection properties declared in the ECCOSORB data sheet.

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 37 ~

International Journal of Material Science

IJMSCI [3]

NRL Tx

[4]

Rx AG ILENT PNA

[5]

[6] [7]

[8]

Tile Fig. 14 Bistatic measurement system located at (www.saslab.eu)

Measurement of the manufactured RAM tile using [9] incidence angle of 0° has been performed for TE and TM mode. In Fig. 14 co mparison between simulation of the reflect ion coefficient of the new manufactured RAM tile and real measurements is shown. The angle of electro magnetic wave incidence is 0°. It can be noticed that the simu lated curve shows similar behaviour with respect to the measured one. Errors and differences in simulated and measured reflect ion coefficient are mainly due to: • difficult ies in manufacturing RAM mult ilayer tile where each layer thickness ranges of about 0.5mm between its minimu m to its maximu m value; so the reported value represent an average value. To be aware of the manufacturing errors, in Fig. 14 we show the measurements of RAM called TE_ 0, TM_0, TE_90, TM_90. The numbers 0 and 90 mean that the RAM tile placed on the metal plate was rotated respectively of 0° and 90°. It can be noticed that there are some differences in the measured reflection coefficients which can be explained by errors in the manufacturing process. • accuracy in determination of permittiv ity of co mposite materials performed using wave guide method. • accuracy in free space measurement of reflection coefficient using bistatic method. V. CONCLUSION In this work modelling, optimizat ion and manufacturing of radar absorbing materials have been discussed. The design and optimization took p lace using the recently introduced winning particle optimizat ion search algorith m wh ich has been applied to optimize the electro magnetic absorbing properties wh ile contemporarily min imizing the overall thickness of mult ilayer material. Following the simu lation, a large t ile of radar absorbing material has been manufactured by using industrial grade of mu ltiwall carbon nanotubes and measurement of electro magnetic reflection coefficient performed by NRL-arch. Co mparison between simu lation and measurement show interesting agreement. Nevertheless some errors occurred in manufacturing process which affected electro magnetic performances of manufactured radar absorbing material. REFERENCES [1] [2]

Lederer, P. G. An Introduction to Radar Absorbent Materials (RAM), Royal Signals and Radar Establishment, Malvern, 1986. Vinoy, K. J.; Jha, R. M. Radar Absorbing Materials: From theory to Design and Characterization, Kluwer Academic Publishers: Boston, 1996.

[10]

[11]

[12] [13] [14]

Knott, E. F.; Shaeffer, J. F.; T uley, M. T. Radar Cross Section, 2Rev. ed ed.; Artech House: Norwood, 1993. Ruck, G. T. Radar Cross Section Handbook; Vol.II, Plenum Press: Newe York, 1970. Andrei Shepelev and Huib Ottens, Horten Ho 229 Spirit of Thuringia: The Horten All-Wing Jet Fighter ,Lan Allan Publishing Ltd, Hersham, Surrey KT12 4RG. 2006. Paul Saville, “ Review of Radar Absorbing Materials”, Defence R&D Canada – Atlantic, 2005. Davide Micheli, Carmelo Apollo, Roberto Pastore,Ramon Bueno Morlesa, Susanna Laurenzi, Mario Marchetti, “Nanostructured Composite Material for Electromagnetic Interference Shielding Applications”, Acta Astronautica, Science Direct, Elsevier, 2011. Davide Micheli, Carmelo Apollo, Roberto Pastore, Ramon Bueno Morles, Daniele Barbera, Mario Marchetti, Gabriele Gradoni, Valter Mariani Primiani, and Franco Moglie, “ Optimization of Multilayer Shields Made of Composite Nanostructured Materials”, IEEE TRANSACTIONS ON ELECTROMAGNETIC COMPATIBILITY, 2011. Davide Micheli, Radar Absorbing Materials and Microwave Shielding Structure Design, LAP Lambert Academic Publishing, 2012. Davide Micheli, Roberto Pastore, Carmelo Apollo, Mario Marchetti, Gabriele Gradoni, Valter Mariani Primiani, and Franco Moglie, “ Broadband Electromagnetic Absorbers using Carbon NanostructureBased Composites”, IEEE Transactions on Microwave Theory and Techniques, 2011. Davide Micheli, Roberto Pastore, Carmelo Apollo, Mario Marchetti, “X-Band microwave characterization of carbon-based nanocomposite material, absorption capability comparison and RAS design simulation”, Composites Science and Technology, 2009. J. A. Kong, Electromagnetic Wave Theory. New York: Wiley, 1986. J. A. Stratton, Electromagnetic Theory. Hoboken, NJ:Wiley-IEEE Press,. 2007. M. H. Umari, D. K. Ghodgaonkar, V. V. Varadan, and V. K. Varadan, “A free-space bistatic calibration technique for the measurement of parallel and perpendicular reflection coefficients of planar samples,” IEEE Trans. Instrum. Meas., vol. 40, no. 1, pp. 19–24, 1991.

Davide Micheli was born in Ancona, Italy, in 1967. He received the University degree in electronics engineering from the University of Ancona (now Università Politecnica delle Marche), Ancona, Italy, in 2001, the University degree in astronautic engineering and Ph.D. in aerospace engineering from the “ Sapienza” University of Rome, Italy, in 2007 and 2011, respectively. He received the University Master degree in composites materials and nanotechnologies in aerospace applications from the “ Sapienza” University of Rome, Italy, in 2012. He is currently with the Telecom Italia Laboratory (TILAB), as a Researcher with Mobile Telecommunications and Neural Networks and collaborates with “ Sapienza” University of Rome, where his research activities are related to EM fields and composite materials interaction. His current research is focused on electric conductive polymers and radar-absorbing structures modeling, manufacturing and testing. Roberto Pastore was born in Naples, Italy, in 1977. He received the University degree in Physics from the University of Studies “ Federico II” of Naples, Italy, in 2003, and the University Master degree in “ Composites Materials and Nanotechnologies for Aerospace Applications” from the “ Sapienza” University of Rome, Italy, in 2006. He’s currently on the Ph.D.Master degree in Aerospace Engineering with “ Sapienza” University of Rome, where his research activities are related to carbon nanoparticles physics and nanocomposite materials characterization. Mario Marchetti was born in San Marcello, Italy, on May 30, 1943. He received the University degree in aeronautical engineering from Milan Polytechnic, Milan, Italy, in 1972. He then joined the School of Aerospace Engineering, “ Sapienza” University of Rome, Rome, Italy, where he is currently a Full Professor of the Engineering Faculty, in charge of the “ Space Structures” course, the Director of the Department of Astronautic, Electric and Energetic Engineering, and is responsible for the SASLab laboratories.

IJMSCI Vol.2 Iss.2 2012 PP.31-38 www.ij-ms.org○ C World Academic Publishing ~ 38 ~

Published on Jun 28, 2012

Modeling of Radar Absorbing Materials Using Winning Particle Optimization

Modeling of Radar Absorbing Materials Using Winning Particle Optimization

Published on Jun 28, 2012

http://www.ij-ms.org Modelling and manufacturing of radar absorbing material are proposed using multilayer composite nanostructured material...

Advertisement